Upload
others
View
10
Download
0
Embed Size (px)
Citation preview
RSC Advances
PAPER
So Condensed Matter, Debye Institute for N
Princetonplein 5, 3584 CC Utrecht, The Net
† Electronic supplementary informa10.1039/c3ra47385f
Cite this: RSC Adv., 2014, 4, 7885
Received 6th December 2013Accepted 7th January 2014
DOI: 10.1039/c3ra47385f
www.rsc.org/advances
This journal is © The Royal Society of C
Predicted stability, structures, and magnetism of 3dtransition metal nitrides: the M4N phases†
Chang-Ming Fang,* Rik S. Koster, Wun-Fan Li and Marijn A. van Huis
The 3d transition metal nitrides M4N (Sc4N, Ti4N, V4N, Cr4N, Mn4N, Fe4N, Co4N, Ni4N, and Cu4N) have
unique phase relationships, crystal structures, and electronic and magnetic properties. Here we present a
systematic density functional theory (DFT) study on these transition metal nitrides, assessing both the
I-M4N phase and the II-M4N phase, which differ in ordering of the N atoms within the face-centered
cubic (FCC) framework of metal atoms. The calculations showed that for M ¼ Mn, Fe, Co and Cu, the
I-M4N phases with perfect metal sub-lattices are favored, while for M ¼ Sc–Cr, and Ni, the II-M4N
phases with distorted metal sub-lattices are favored. We predict that several currently not existing
II-M4N phases may be synthesized experimentally as metastable phases. From Bader charge analysis
the M4N phases are found to be ionic with significant metal–metal bonding. I-M4N with M ¼ Cr to
Ni are magnetic, while II-M4N with M ¼ Cr and Ni are non-magnetic. The calculations revealed
unusually high local magnetic moments and high spin-polarization ratios of the M1 atoms in I-M4N
(M ¼ Cr to Ni). The origin of magnetism and lattice distortion of the M4N phases is addressed with
the Stoner criterion. Detailed information about the relative stability, structures, chemical bonding,
as well as the electronic and magnetic properties of the phases are of interest to a wide variety of
fields, such as chemical synthesis, catalysis, spintronics, coating technology, and steel manufacturing.
Fig. 1 Schematic structure for I-M4N (a, left) and II-M4N (b, right). Theblack bold-lines indicate the axis of the unit cell. The octahedrally-
1. Introduction
The interest in the M4N transition metal nitrides is multifold.First, M4N nitrides with M ¼ Fe, Co and Ni, have unique elec-tronic andmagnetic properties and consequently have potentialapplications as magnetic recording materials,1–5 as spin carriersin spintronics3–6 and even as catalysts used for photocatalyticwater splitting.7
Second, there are two possible phases for M4N (the I-phaseand the II-phase) that are structurally difficult to distinguish butthat can have very different physical properties. In the early1960s, Terao observed two Ni4N phases.8,9 One of them is cubic(I-M4N with M ¼ Ni),8 and has a conventional face-centeredcubic (FCC) cell with one N atom at the center. Within this I-phase, there are two crystallographically different sites for themetal atoms in the FCC-sub-lattice: one is at the corner with 12metal atomic neighbors, and the other three are at the facecenters, each of which has 12 metal neighbors and two N atomneighbors, as shown in Fig. 1. The two types of metal atoms inthis phase have signicantly different characteristics, whichleads to interesting electronic and magnetic properties.2–7
anomaterials Science, Utrecht University,
herlands. E-mail: [email protected]
tion (ESI) available. See DOI:
hemistry 2014
The second Ni4N phase that Terao found (II-M4N withM ¼ Ni) is tetragonal with a � a0 and c # 2a0 (here a0 is thelattice parameter of cubic I-M4N).9 Compared to the cubic I-M4N
coordinated N atoms form a simple cubic lattice in I-M4N with twocrystallographically different M atoms: M1 at the corners of the cell,coordinated by 12 M2 atoms, and three M2 atoms at the face centers,coordinated by four M1, 8 M2 atoms and 2 N atoms. In II-M4N, theoctahedrally-coordinated N atoms form a body-centered tetragonalstructure with also two M species: M1 in the planes z ¼ 0 and z ¼ 1/2,each M1 coordinated by 4 M1, 8 M2 and 1 N atoms, M2 at zz 1/4 and zz 3/4, whereby each M2 has 8 M1, 4 M2 and 2 N neighboring atoms.
RSC Adv., 2014, 4, 7885–7899 | 7885
RSC Advances Paper
phase with a perfect FCC metal sublattice, in the tetragonalII-M4N phase the FCC metal sublattice is distorted, and hastwo N atoms at octahedral sites, as shown in Fig. 1.9 Up tonow most studies are on the I-type structures. There are veryfew papers on the II-phases. Throughout rest of this manu-script, we use the denitions by Terao.8,9 It is of generalinterest to explore the relative stability, structures andunique electronic properties of these two M4N phases.
Third, the itinerant nature of 3d transition metals and therelated compounds has been a fascinating topic for solid statescientists for over half century.10–15 Although intensive investi-gations have been performed for the 3d transition metals11,12
and ionic transition compounds, such as the oxides,13–15 thereare much fewer studies on the 3d transition metals of partialoxidation, which is the case for 3d transition metal sub-nitrides,M4N (M ¼ 3d transition metals).14–16 Furthermore, the magne-tism and its origin for the M4N phases are of great interest forscientists in the elds of physics, chemistry and materialsscience.
Experimentally, most M4N samples have been prepared forM ¼ Mn, Fe, Co and Ni in the forms of e.g. powder by nitrid-ization of the metals,1–9,16–18 as thin-lms by sputtering tech-niques3,4,19 and as nanoparticles on substrates by molecularbeam epitaxy techniques.20 In general, it is difficult to obtainpure samples with high homogeneity using these methods.That has an impact on the accuracy and reliability of theexperimental assessments of the physical properties. Therefore,much remains to be claried. For example, Blucher and co-workers reported I-Cu4N samples they prepared by means of DCplasma ion nitridization. They found a lattice parameter ofabout 3.19 A, which is much smaller than that (�3.61 A) of pureFCC-Cu.21
To resolve such issues theoretical methods, especiallyparameters-free rst-principles methods, are very useful. Therst-principles density-functional theory (DFT) approaches havebeen used for I-M4N, in particular for M ¼ Fe.22–32
With the assumption that the lattice parameters of thetetragonal II-Fe4N are a¼ a0, c ¼ 2 a0 (a0 is the lattice parameterof cubic I-Fe4N), Kong and co-workers performed electronicband structure calculations using the rst-principles LinearMuffin-Tin Orbital (LMTO)method and addressed the inuenceof N ordering on the electronic and magnetic properties of M4N(M ¼ Fe) with the two I- and II-phase structures and observed astrong impact of local crystal structure on the local magne-tism.25 Mohn and co-workers studied the magnetic and elec-tronic properties of I-M4N with M ¼ Mn and Fe and observedferro-magnetic (FM) nature for M ¼ Fe and ferri-magnetic (FR)ordering for M ¼ Mn.33,34 Matar and co-workers studied themagnetic properties of cobalt metal and tetra-cobalt nitride (I-M4N withM¼ Co).35 From the dispersion curves, Takahashi andco-workers6 explored the electronic and magnetic properties ofternary I-(M1�xM0
x)4N, (M ¼ Co, M0 ¼ Fe) compounds. Theyobserved a nearly half-metallic electronic structure for I-Co4N,and a half-metallic behavior for I-(Co1�xFex)4N, whereby atx ¼ 1/4 the energy gap is about 0.2 eV for the spin-up (majority)electrons. That suggests that this material has potential appli-cation as spin-carrier materials for spintronics devices.6,36–40 In
7886 | RSC Adv., 2014, 4, 7885–7899
the rst-principles' study of stability and electronic andmagnetic properties of nickel nitrides, Fang and co-workersrevealed that I-Ni4N is magnetic while I-Ni4N1�x (x� 0.1) phasesare non-magnetic due to the distortion of the FCC Ni sub-latticecaused by extra/deciency of N atoms.41 More theoreticalstudies were conducted on the electronic and magnetic prop-erties of ternary I-(AxM1�x)4N phases where A is a metallicelement and M a 3d transition metal.6,42–46 Dos Santos and co-workers performed structural optimization and electronic bandstructure calculations for a novel I-M4N (M ¼ V) phase.47 Upto now, theoretical calculations have been performed mainly forI-M4N with M ¼Mn, Fe, Co, Ni and Cu,22–41,48,49 and there is lackof knowledge about the formation and stability, and physicalproperties of the II-M4N phases.
In the present manuscript, we present a systematic rst-principles study on the stability, the structure, and the elec-tronic and magnetic properties of I- and II-M4N (M ¼ Sc to Cu)phases. The trends in chemical bonding, valence and chargetransfer in the M4N were addressed together with the electro-negativity of the 3d transition metals. The (in-)stability ofparamagnetic I-M4N phases was investigated using the Stonertheory.10–12,50,51 The obtained information here is important notonly for solid state scientists to understand the nature of 3dtransition metals and related compounds, but also for experi-mentalists for obtaining a reliable characterization of preparedsamples and to understand the physical properties of the binaryM4N and ternary (M,M0)4N phases, many of which are meta-stable.20,21,52 Finally, the calculated results are of interest for thedevelopment of applications in various elds, such as chemicalsynthesis,1–9,16–18 coating,19,20 catalysis,7 spintronics,6,36–40 andsteel manufacturing.53,54
The article is arranged as follows. In the following Section(2), we introduce the criteria used to assess the stability of thenitrides (formation energy) with respect to the elemental metalsand a N2 molecule (2.1). Next the Bader charge analysisapproach used in the present work is described in Section 2.2.Details of the rst-principles density-functional theory (DFT)techniques and settings are described in Section 2.3. Section 3(Computational results and discussion) starts with theelemental metals (3.1), followed by the stability, structuralproperties, chemical bonds, and charge transfer in the M4Nphases (3.2). The electronic and magnetic properties of the M4Nphases are described in 3.3. Finally, in Section 3.4 we addressthe origin of magnetism and phase stability of M4N usingStoner criterion together with the FCC-3d elemental metals.Finally a brief summary of the calculations and results is pre-sented in Section 4.
2. Details of calculations2.1. Formation energy
The formation energy (DE) of a metal nitride with the formula,M4N, M ¼ Sc to Cu with respect to the elemental 3d transitionmetal M and the N2 molecule can be described as:41,54,55
DE(M4N) ¼ E(M4N) � [4E(M) + E(N2)/2] (1)
This journal is © The Royal Society of Chemistry 2014
Paper RSC Advances
here, E(M4N), E(M) and E(N2) are calculated using the DFT-GGAapproach (see below). This energy difference, DE(M4N) is inunits of eV per M4N (eV/f.u.) and can be used to assess therelative stability of the M4N phases. Positive values meanmetastable and negative values indicate stable with respect tothe elemental metal and N2 gas. At 0 K and 0 Pa, the enthalpydifference is equal to the energy difference, that is DH(M4N) ¼DE(M4N), where we ignore the zero-point vibrationcontribution.
2.2. Bader charge and charge transfer in crystals
One of the difficulties in solid state science is the denition ofthe shape and volume of an atom or ion and correspondinglythe charge on and charge transfer from/to the atom/ion in asolid.56 In 1971, Bader and Beddal proposed a unique denitionof an atom/ion in a molecule/solid by dividing the molecule/solid into spatial regions dening the atoms, and the charge onthe atom is determined by the number of electrons in eachregion.56,57 The boundary of an atom is dened by the zero-uxsurfaces between that atom and neighboring atoms. That is, thecharge density distribution r(r) is partitioned by the closesurface, S(r), through which the ux density Vr(r) is zero,
Vr(r)$n(r) ¼ 0 (2)
where the ux density Vr(r)¼ (v/vx, v/vy, v/vz)r(r) is a vector andn(r) is the unit vector normal to the surface S(r) at r. This de-nition is sufficient to unambiguously partition any molecular orcondensed matter system of a nite or innite size. Then thenumber of electrons in the volume centered by a density peak(nucleus or ion of atom A) can be obtained by integrating theelectron density in the volume bounded by S(r),
N(A) ¼ Ðr(r)dr (3)
and the charge for ion A with Z valence electrons is obtainedfrom
Q(A) ¼ Z – N(A) ¼ Z � Ðr(r)dr (4)
Henkelman and co-workers58 implemented Bader chargeanalysis into different rst-principles DFT codes, including theVienna Ab initio Simulation Package (VASP).59,60 The Badercharge approach has been widely used in ab initio studies ofchemical reactivity of atoms/ions in molecules or solids.37,58,61
2.3. Details of rst-principles calculations
The rst-principles code VASP59,60 was used for all the calcula-tions. This code employs Density-Functional Theory (DFT)within the projector-augmented wave (PAW) method.62,63 Thegeneralized gradient approximation (GGA) formulated by Per-dew, Burke and Ernzerhof (PBE)64 was employed for theexchange and correlation energy terms because the GGAapproximation describes (spin-polarized) transition metals andcompounds better than the local (spin-polarized) densityapproximation.65,66 We remark here that the small number ofvalence electrons of elements, especially those of the rst half
This journal is © The Royal Society of Chemistry 2014
column in the periodic table, has an impact on the calculationsof Bader charges at atomic sites in a crystal.58,61 To obtain reli-able values of Bader charges in the M4N phases, we also usedthe potentials (M_pv) containing semi-core 3p6 elec-trons.59,60,63,64 Our test-calculations showed that using the PBE-GGA potential with/without the semi-core 3p6 electronsproduced no notable differences in the results on crystalstructure, total energy differences, and electronic and magneticproperties. The cut-off energy of the wave functions was 550 eV.The cut-off energy of the augmentation functions was 700 eV. A2a0 � 2a0 � 2a0 supercell is used for I-M4N (a0 is the latticeparameter of the cubic cell) to facilitate the integration ofcharges/electrons in the atomic spheres. The electronic wavefunctions were sampled on a 12 � 12 � 12 grid with 84k-pointsand 24 � 24 � 12 grid with 468k points in the irreducibleBrillouin zone (BZ) of the 2a0 � 2a0 � 2a0 super-cell of I-M4Nand the conventional cell of II-M4N, respectively, using theMonkhorst–Pack method.67 Dense k-meshes were used for theelemental 3d transition metals as well. For the calculations oflocal electronic congurations and partial density of states ofthe atoms, theWigner–Seitz radius is set at 1.4 A for M and 1.0 Afor N, respectively, considering the metallic nature of thenitrides. Note that the M 3d electrons exhibit an itinerantcharacter in the metals and their nitrides, and in principlebelong to the whole crystal. However, we can decompose theplane waves in the sphere and obtain M 3d components in thespheres for both the spin-up (or majority) and spin-down(minority) directions. In this way a local magnetic moment isobtained which is the difference of the number of spin-upelectrons and spin-down electrons in the sphere. Different k-meshes and cut-off energies for the waves and augmentationwaves were tested. The settings mentioned above ensure a goodconvergence (�1 meV per atom).
3. Computational results anddiscussion3.1. Structure of the elemental 3d metals
As shown in eqn (1), in order to obtain the formation energies ofthe nitrides it is required to rst calculate the total valenceelectron energies of a N2 molecule and the stable elementalsolids with the same technique and settings in Section 2.3.Calculations for the N2 molecule were performed in a large cubewith axis length a ¼ 12 A.61 The cut-off energy of the wavefunctions of 1000 eV was employed to describe the stronglylocalized 2p bonds of the N2 molecule. The calculated bond-length is 1.11 A, comparable to the experimental value (1.10 A).
The 3d transition metals have been studied inten-sively.10–12,50,68–73 It has been recognized that 3d transition metalatoms have the unique 3dn4s2 with n ¼ 1 to 10 (from Sc to Zn)with two exceptions, Cr 3d5 4s1 and Cu 3d10 4s1. The exceptionsoriginate from the preference of half (3d d5 for Cr) and fulloccupations (3d10) of the 3d states.73,74 As shown in Table 1, theground state of elemental Sc, Ti, Co and Zn metals has a hexag-onally-closed-packing (HCP) lattice, V, Cr and Fe a body-centeredcubic (BCC) lattice, Ni and Cu a faced-centered cubic (FCC)
RSC Adv., 2014, 4, 7885–7899 | 7887
Table 1 Calculated results (lattice parameters, local magnetic moments) of the elemental 3d transition metals from first-principles DFT-GGA.Available experimental data from the literature are included for comparison
c_Pauling116/c_Allen
117
Present calculations Experiments in literature
Latt. para. (A) Magn. Latt. para. (A) Magn.
HCP-Sc 1.36/1.19 a ¼ 3.320 NM 3.309 (ref. 69) NMc ¼ 5.164 5.273
HCP-Ti 1.54/1.38 a ¼ 2.924 NM 2.9508 (ref. 69) NMc ¼ 4.626 4.6855
BCC-V 1.63/1.53 a ¼ 2.979 NM 3.03 (ref. 69) NMBCC-Cr 1.66/1.65 a ¼ 2.855 AFM � 1.06 2.8787 (ref. 68) FRM (ref. 71 and 77), 0–1.30
2.91 (ref. 69)BCCa-Mn 1.55/1.75 a ¼ 8.605 FRMa, 0–2.9 8.877 (ref. 72) FRM (ref. 72 and 75), 0–2.9
c ¼ 8.604 8.873BCC-Fe 1.83/1.80 a ¼ 2.833 FM 2.21 2.8665 (ref. 68) FM,79 2.17
2.8607 (ref. 69)HCP-Co 1.88/1.84 a ¼ 2.496 FM, 1.63 2.5071 (ref. 69) FM (ref. 80 and 82), 1.60
c ¼ 4.033 4.0695FCC-Ni 1.91/1.88 a ¼ 3.524 FM, 0.63 3.5175 (ref. 68) FM,78 0.60
3.524 (ref. 69)FCC-Cu 1.90/1.85 a ¼ 3.637 NM 3.6149 (ref. 68) NM
3.6077 (ref. 69)HCP-Zn 1.65/1.59 a ¼ 2.650 NM 2.6649 (ref. 69) NM
c ¼ 5.046 4.9468N (N2) 3.04/3.066 d(N–N): 1.11 d(N–N): 1.10
a BCC-type cell with 58 Mn atoms, and ferrimagentic (FRM) ordering with absolute values of moments ranging from 0.0 to 2.8372-75, see the text fordetails. Here NM represents non-magnetic, AFM anti-ferromagnetic and FM ferromagnetic.
RSC Advances Paper
lattice.68–73 Elemental Mnmetal has a complicated crystal structureat ground state.72–75 Obviously, there have beenmany experimentaland theoretical efforts on the structural, electronic and magneticproperties of 3d transition metals.10–14,50,51,68–75 However, here theexperimental values servemerely as a reference for the calculationson the nitrides, therefore, we limit ourselves to comparison withthe available experimental observations in literature.
The early transition metals Sc, Ti and V are non-magnetic.Elemental Cr has a simple BCC structure,68,69 but a complexspiral-like magnetic ordering.70,71 In the present calculations welimit ourselves to the anti-ferromagnetic ordering with one layerof Cr atoms being magnetically opposite to the neighboringlayer ones, considering the small energy differences betweenthe spiral magnetic ordering and AFM ordering.70,71
The calculations also showed that the non-magnetic (NM)solution has just a slightly higher energy (about 10 meV/Cr). Thatagrees with the complex magnetic behavior of Cr metal.11,12,68–72
There are also discussions about the ground state of Co.11,35
Therefore, we also performed structural optimization and totalenergy calculations for HCP-, BCC- and FCC-Co. The calculationsshowed that all the three phases being ferromagnetic (FM) withthe order of stability: HCP-Co (set dE¼ 0.0 eV/Co) > FCC-Co (dE¼+0.019 eV/Co) > BCC-Co (dE ¼ +0.099 eV/Co), in agreement withthe experimental observations68,69,76 and the former theoreticalcalculations.11,35,74 The calculated magnetic moments (1.60 mB/Cofor HCP-phase, 1.64 mB/Co for FCC-phase, and 1.74 mB/Co for BCC-phase) are close to the former calculations (1.63 mB/Co for HCP-phase, 1.67 mB/Co for FCC-phase, and 1.76 mB/Co for BCC-phase)by Matar and co-workers using the all electron augmented spher-ical wave (ASW) method.35 The crystal structure and magnetic
7888 | RSC Adv., 2014, 4, 7885–7899
ordering of pure Mn have been a topic of interest. Both experi-mental and theoretical studies showed the dependence of crystalstructure on its spiral-like magnetic structure.72,75 Here we use asimplied ferrimagnetic (FR) ordering model to optimize itsstructure and to obtain total valence electron energy as a refer-ence.75 Our calculations provide a solution with a nearly cubiclattice which agrees with the experimental values within 1% (asshown Table 1). The obtained localmagneticmoments are: Mn1 (2atoms) 2.98 mB, Mn2 (8 atoms) �2.27 mB, Mn3 (24 atoms) 0.47 mBandMn4 (24 atoms)�0.12 mB. The calculated localmoments are inagreement with the experimental values (e.g. the absolute values,Mn1 2.83 mB, Mn2 1.83 mB, Mn3 0.5 to 0.6 mB and Mn4 0.45 to 0.48mB by Lawson et al.72), considering the strong dependence of the(spiral) magnetism on temperature, impurity, etc. In fact assummarized by Hobbs and co-workers, both experimentalmeasurements and theoretical calculations provide a signicantvariety of local moments.75 Therefore, the present calculationsprovide one ferrimagnetic solution with reasonable stability.
Overall, the calculated lattices of the 3d transition metals arein good agreement with the experimental values (<2%, Table 1).The calculated local magnetic moments for AFM BCC-Cr, FR a-Mn (a BCC-type cell), and FM BCC-Fe, FM HCP-Co and FM FCC-Ni are close to the available experimental values and formertheoretical calculations in literature.12,68–82
3.2. Stability, structural properties and chemical bonding ofthe M4N phases
As shown in Fig. 1, I-M4N has a perfect M FCC sub-lattice withone N atom occupying one of the octahedral sites. The N atoms
This journal is © The Royal Society of Chemistry 2014
Fig. 2 Formation energies (DEform) of I- (filled black spheres) and I-M4N phases (filled red squared) with respect to the nonmagnetic I-M4N. Clearly, I-M4N phases aremore stable than II-M4N for M¼Mn, FeCo and Cu. Meanwhile, for M ¼ Sc, Ti, V Cr, Ni (and Zn), the II-M4Nphases are favored over the corresponding I-M4N phases. The dottedlines are drawn to guide the eyes.
Paper RSC Advances
also are a simple cubic lattice in the I-phases. It shouldbe realized that due to the magnetic ordering, the symmetry ofI-M4N (M ¼ Cr, Mn, see 3.3) is lowered into a tetragonal sub-lattice. In the II-M4N phases, the N atoms form a body-centered tetragonal sub-lattice (BCT). This arrangement allowsthe M FCC sub-lattice to become one face-centered tetragonal(FCT) lattice.
Table 2 lists the calculated lattice parameters and formationenergies for the M4N phases. Fig. 2 shows the stability of the I-and II-M4N phases relative to the corresponding non-magneticI-phases according to Table 2. Table 3 lists the calculated latticeparameters for non-magnetic FCC-3d transition metals,nonmagnetic and magnetic I-M4N, and for II-M4N.
For the cubic I-M4N, the structure is determined by its latticeparameter a. For the tetragonal I-type phases, two latticeparameters a and c are required. However, the fractional atomiccoordinates are the same: one N at (1/2,1/2,1/2); one M1 at(0,0,0), and three M2 at (1/2,0,1/2), (0,1/2,1/2) and (1/2,0,1/2) asshown in Fig. 1. For the tetragonal II-M4N phases which havetwo lattice parameters a and c (�2a), the fractional coordinatesof atoms are: N at (0,0,0), and (1/2,1/2,1/2); M1 at (0,1/2,0), (1/2,0,0), (0,1/2,1/2) and (1/2,0,1/2); M2 at (0,0,z), (0,0,�z), (1/2,1/2,1/2 � z) and (1/2,1/2,1/2 + z) with z � 0.25.
Note that in the schematic structure of II-M4N in Fig. 1the origin is shied with z � 0.25 with respect to the
Table 2 DFT-GGA calculation results (lattice parameters, local magnetiAvailable experimental and selected former theoretical calculations are iM2. FR-II indicates one layer antiparallel to neighboring layers along z-axatoms in the neighboring two layers
I-M4N
Latt. para. (A) Magnetism DE(eV)
Sc4N 4.555 NM �2.980
Ti4N 4.162 NM �3.624
V4N 3.920 NM �2.208(3.979)47
Cr4N 3.776 NM �0.3293.814 FR-I �0.463
Mn4N 3.696 NM �0.0803.849 FR-I �0.758(3.864)97,98
3.740 FR-II3.783 (See text) �0.768
Fe4N 3.672 NM 1.1343.793 FM �0.205(3.790)18
Co4N 3.685 NM 1.3183.728 FM 0.415(3.738)25
Ni4N 3.733 NM 0.5093.739 FM 0.470(3.72)8
Cu4N 3.877 NM 1.531(3.193)21
Zn4N 4.1797 NM 1.912
This journal is © The Royal Society of Chemistry 2014
abovementioned fractional coordinates of atoms. The struc-tural optimizations provide the z-coordinates for M2 atomsas follows, z(Sc2) ¼ 0.2265 (II-Sc4N), z(Ti2) ¼ 0.2416 (II-Ti4N),z(V2) ¼ 0.2783 (II-V4N), z(Cr2) ¼ 0.2650 (II-Cr4N), z(Mn2)¼ 0.2572 (II-Mn4N), z(Fe2) ¼ 0.2597 (II-Fe4N), z(Ni2) ¼ 0.2545(II-Ni4N), z(Cu2) ¼ 0.2600 (II-Cu4N), and z(Zn2) ¼ 0.2551 (II-Zn4N). It is clear that for M ¼ Sc, Ti, the neighboring M2atoms tend to approach the N atoms.
c moments and formation energies from eqn (1)) for the M4N phases.ncluded for sake of comparison. FR-I indicates M1 being antiparallel tois. FR-III indicates two layers of metal atoms anti-parallel to the metal
II-M4N
Latt. para. (A) Magnetism DE(eV/f.u.)
4.470 NM �3.3899.7114.145 NM �3.7018.4924.128 NM �2.6726.8323.832 NM �0.6287.1613.829 FR-III �0.6597.446
3.782(3.792)25 FM �0.1457.368(7.584)25
3.731 FM 0.4747.369
3.760(3.72)9 NM 0.3067.271(7.28)
3.887 NM 1.6967.6474.0887 NM 1.7578.7043
RSC Adv., 2014, 4, 7885–7899 | 7889
Table 3 Inter-atomic distances for cubic I-M4N, tetragonal I-M4N due to ferrimagnetism (FRM), and tetragonal II-M4N phases. The fractionalcoordinates of atoms in I-M4N are: one N at (1/2,1/2,1/2); one M1 at (0,0,0), and three M2 at (1/2,0,1/2), (0,1/2,1/2) and (1/2,0,1/2) as shown inFig. 1. For the tetragonal II-M4N phases which have two lattice parameters a and c (�2a), the fractional coordinates of atoms are: N at (0,0,0), and(1/2,1/2,1/2); M1 at (0,1/2,0), (1/2,0,0), (0,1/2,1/2) and (1/2,0,1/2); M2 at (0,0,z), (0,0,� z), (1/2,1/2,1/2� z) and (1/2,1/2,1/2 + z) with z� 0.25. Note, inthe schematic structure of II-M4N in Fig. 1, the origin is shifted with z � 0.25
System Lattice M1– distance to M2– distance to N– distance to
I-M4N Cubic a M2: O2a/2 (�12) N: a/2 (�2) M2: a/2 (�6)M1: O2a/2 (�4)M2: O2a/2 (�8)
I-M4N Tetragonal a, c M2: O(a2 + c2)/2 (�12) N: a/2 (�1) M2: a/2 (�4)c/2 (�1) c/2 (�2)M1: O(a2 + c2)/2 (�4)M2: O2a/2 (�4)O2c/2 (�4)
II-M4N Tetragonal a, c N: a/2 (�2) N: zc (�1) M1: a/2 (�4)M1: O2a/2 (�4) M1: O{a2+[zc]2}/2 (�4) M2: zc (�2)M2: O{a2 + (zc)2}/2 (�4) O{a2+[(1/2 � z)c]2}/2 (�4)O{a2+[(1/2 � z)c]2}/2 (�4) M2:O2a/2 (�4)
RSC Advances Paper
The very short c-axis in II-V4N causes repulsion of M2 atomsfrom the N atoms with a signicantly large z(V2) value. For theother II-M4N phases, the M2 atoms shi away moderately fromthe N atoms with z(M2) ranging from 0.255 (M ¼ Zn) to 0.265(M ¼ Cr).
We started from the lattice parameters for the 3d transitionmetals with a non-magnetic solution (Fig. 3). The latticeparameters change smoothly with the atomic number in a valleyshape: they decrease from Sc to Fe and then increase to Zn. Asshown in Fig. 3, the dependence of the a lattice parameter ofnon-magnetic I-M4N on the atomic number of the metals is verysimilar to that of the nonmagnetic FCC-metals, with somedifferences: except for M ¼ Sc, the lattice parameters of thecubic non-magnetic I-M4N phases are larger than those of cor-responding FCC metals. This is due to the atomic volume of Natoms in the lattices.
Magnetism has a strong impact on the lattice parameters ofthe I-M4N phases. For M ¼ Sc–V, the I-M4N phases are non-magnetic. For M ¼ Cr and Mn, the I-M4N phases have ferri-magnetic ordering, and as a consequence the lattices becometetragonal with a being identical for M ¼ Cr (a pseudo-cubiclattice), and c/a being equal to 1.011 for M ¼Mn. For M ¼ Fe to
Fig. 3 Calculated lattice parameters for non-magnetic FCC-3d tran-sition metals (open black circles), nonmagnetic I-M4N (red soldsquares), magnetic I-M4N (red diamonds) and a-axis (green solidtriangles up) and half the c-axis (solid triangles-down) of II-M4N. Linesare drawn to guide the eye.
7890 | RSC Adv., 2014, 4, 7885–7899
Ni, the I-M4N phases are ferromagnetic and cubic with theirlattice parameters larger than the corresponding non-magneticlattices. The last two the I-M4N phases with M ¼ Cu and Zn arenon-magnetic.
The high symmetry of cubic I-Mn4N phases gives a simplegeometrical relationship for calculating the bond lengths in thestructures: each M1 has 12 M2 neighbors with a bond length ofO2a0/2 (a0 is the lattice parameter), while each M2 atom has4 M1 and 8 M2 nearest neighbors with the same bond length,and 2 N neighbors with a M–N distance of a0/2. Meanwhile therelationships between the chemical bonds and lattice parame-ters become more complicated with distortions of the latticesfor tetragonal I-M4N due to magnetism (M ¼ Cr, Mn). Nordering also causes distortion of the II-M4N lattices. We list therelationships for the different M4N phases in Table 3.
Fig. 3 also shows the lattice parameters for the II-M4N pha-ses. For sake of comparison we plot c/2, as shown in Fig. 1. Asshown in Table 2, the length of a-axis is smaller than that of c/2for Sc and Ti. This relationship changes dramatically whenM ¼ V and for the other M ¼ 3d metals the c/2a values aresmaller than 1. Here we divide the M4N phases into fourdifferent species according to their characteristics, as discussedbelow.
3.2a. M ¼ Sc–V. The calculations showed that both I- andII-M4N phases are stable relative to the elemental metal and theN2 molecule, with the II-phases being favored over I-M4N. Forthe calculated lattices, there is a strong change in the latticeparameters: for M¼ Sc and Ti, the a-axis of II-phases are shorterthan those of the corresponding I-phases. The c/2a rations arelarger than 1, in contrast to the M¼ V phases where II-V4N has alonger a-axis and a small c/2a ratio, as shown in Table 2.
The calculations also showed that II-Sc4N has a slightlyshorter a-axis than that of I-phase, and a large c/2a ratio(¼1.086). Total energy calculations showed that both Sc4Nphases have higher stability with respect to the elemental HCP-Sc and the N2 molecule (Table 2). The situation for the Ti4Nphases is very similar to that of Sc4N, as shown in Table 2 andFig. 2 and 3. There are also some differences. The calculations
This journal is © The Royal Society of Chemistry 2014
Paper RSC Advances
show a smaller energy difference between the I- and II-phases.The c/2a ratio being 1.024 for II-Ti4N is less signicant than thatfor I-Sc4N. The fractional atomic coordinates (z ¼ 0.2265 for II-Sc4N and z ¼ 0.2416 for II-Ti4N) are smaller than 0.25. Thatindicates that the M2 atoms/ions are attracted to N atoms,which stabilizes the two II-phases.
Both V4N phases show high stability relative to the elementalBCC-V and N2, as mentioned above. Comparatively, the calcu-lations showed a signicantly different behavior for the V4Nphases: an a lattice parameter (4.128 A) for the II-phase that ismuch larger than that (3.920 A) of I-V4N; and a small c/2a ratiobeing equal to 0.83 for II-V4N. The calculated lattice parameterfor I-V4N is close to that (3.984 A) of the former work by dosSantos and co-workers, the only paper for I-V4N found in liter-ature.47 The calculations also show that both V4N are non-magnetic, in agreement with the former calculations.47 Thesignicant lattice changes (long a-axis and short c-axis) are theorigin of stabilization of the II-V4N phase.
The calculations showed that the M4N (M¼ Sc–V) phases arestable relative to the elemental solids and nitrogen gas (Table 2).However, there are no experimental observations for the above-mentioned phases.82–93 The stable binary compound in the Sc–Nsystem is ScN with NaCl-type structure which has an FCC-Scsub-lattice.82,83 We performed rst-principles calculations forScN and obtained a ¼ 4.518 A, in good agreement with therecent experimental value, 4.5005 A.83
From the equation: Sc4N(s) ¼ 3Sc(s) + ScN(s) + DHform, thenDHform¼ +0.855 eV/f.u. for I-Sc4N and +0.446 eV/f.u. for II-Sc4Nunder the conditions T¼ 0 K and p¼ 0 Pa, with the ignoring ofzero-vibration contributions. This indicates that both I- and II-Sc4N phases are metastable with respect to rocksalt ScN andHCP-Sc metal. This conclusion agrees with the experimentalobservation.82,83 For titanium and vanadium nitrides, we alsotried to compare the stability of M4N phases relative to thewell-known MN phases with the reactions: M4N(s) ¼ 3M(s) +N(s) + DHform, and found that DHform ¼ �0.505 eV for II-Ti4Nand DHform ¼ �0.759 eV for II-V4N. However, it has been well-established that there are chemical non-stoichiometriccompounds, e.g. d0-MN1�x with FCC-M sub-lattices with de-ciency x being as high as about 0.4.84–93 The defective struc-tures contain signicant contributions from congurationalentropy for the reactions typically taking place at elevatedtemperatures. Simple solid reactions are not available due tothe interplay of complex crystal structures and defects.Meanwhile, the possibility to form II-M4N (M¼ Ti and V) couldnot be excluded. These systems are worth futureinvestigations.
3.2b. M ¼ Cr and Mn. The M4N phases with M ¼ Cr andMn are calculated to be more stable than the elemental solidand N2. Both elements in the M4N phases exhibit uniquemagnetic properties. The two elements have different inu-ences on the phase relations (Table 2 and Fig. 2).
The calculations showed that magnetism lowers theformation energy of I-Cr4N by about 0.34 eV/f.u. (Fig. 2) Themagnetism also reduced the symmetry of I-Cr4N into tetrag-onal with almost identical lengths of the a- and c-axis (pseudo-cubic). Meanwhile, the II-phase is calculated to be non-
This journal is © The Royal Society of Chemistry 2014
magnetic, with its formation energy about 0.156 eV/f.u. lowerthan that of the magnetic I-phase (Fig. 2). There are severalbinary compounds in the Cr–N binary phase.94,95 One of themis CrN with zinc-blende structure. We performed total energycalculations for CrN with NaCl-type structure. The calculationsusing the anti-ferromagnetic ordering produced lattice parame-ters a¼ 4.1435 A and c¼ 4.1267 A, with a localmagneticmomentof 2.358 mB/Cr.
Experimentally, Aoki and co-workers prepared CrN samplesat high temperature with a cubic lattice (a ¼ 4.146 A).96
Considering the magnetic effects, our calculated CrN latticesare close to the experimental values.96 Using the formula:Cr4N(s)¼ 3Cr(s) + CrN(s) + DHform, we obtained DHform¼ +0.356eV for I-Cr4N and + 0.205 eV for II-Cr4N. Therefore, both I- andII-Cr4N phases are metastable with respect to CrN and BCC-Crsolids.
An even larger effect of magnetism on the formation energyis observed for I-Mn4N (Fig. 2). Two solutions have beenobtained for I-Mn4N: one FR-I with the magnetic moments ofMn1 anti-parallel to those of M2 atoms. Another one is withone layer of M atoms anti-parallel to the neighboring layers.The calculations show only a very small energy difference(about 10 meV/f.u.) (Table 2). Therefore, we expect that morecomplex magnetic orderings are possible within the structure,without signicant energy differences. The calculated latticeparameter for I-Mn4N is close to the experimental value within1%, as shown in Table 2.97–99 Mohn and co-workers also per-formed electronic structure calculations for I-Mn4N with theexperimental lattice parameter and also obtained a FR-Iordering.34 Similar results were obtained by Siberchicor andMatar.33 Our calculations also showed that the lattice of I-phase is slightly more stable than the II-phase with an energydifference of 0.110 eV/f.u. Such a small energy difference alsoindicates the possibility of co-existence of the two phases atelevated temperature, considering that only the Mn4N phasewith presumed I-type structure has been preparedexperimentally.97,98
3.2c. M ¼ Fe, Co and Ni. Although the ground state of themetastable FCC-Fe has a spiral magnetic structure,100 additionof carbon or nitrogen can induce ferro-magnetism.101 The M4N(M ¼ Fe, Co and Ni) phases are expected to have ferromagneticordering from the available experimental measurements andtheoretical simulations.1–9,17–35 The cubic symmetry for the I-M4N is then retained and is determined by its lattice param-eter a (Table 2 and Fig. 3). The calculated structures agree wellwith the experimental data for M¼ Fe–Ni, as shown in Table 2.Kong and co-workers performed electronic structure calcula-tions for II-Fe4N by assuming lattices a ¼ a0 (lattice parameterof I-type structure) and c ¼ 2a.25 The calculated latticeparameter for I-Co4N is close to the experimental value (3.738A),103,104 and is much larger than the experimental value (3.587A) by Oda and co-workers.105 The small lattice parameter mayoriginate from N deciency.35 Our calculated lattice parameterfor I-Co4N is also close to the value of 3.737 A by Matar and co-workers who used the DFT-GGA scheme.35 The magnetismleads to a slight volume increase of the I-M4N phases. Both I-and II-type phases are ferromagnetic and the I-type structure
RSC Adv., 2014, 4, 7885–7899 | 7891
Fig. 4 Bader charges at the different metal sites (top), and N ions(bottom) (also see Table S1†). The differences (Dc) between theelectronegativity of a metal and that of N for the two sets of electro-negativity of 3d transition atoms with the formula, Dc ¼ c(M) – c(N),are also included for sake of comparison. Lines are drawn to guide theeye.
RSC Advances Paper
has a higher stability (Table 2). The calculations showed that I-Ni4N is magnetic while II-Ni4N is non-magnetic and is morestable than the I-type lattice.
The calculations give a formation energy of�0.205 eV/f.u. forI-Fe4N and �0.145 eV/f.u. for II-Fe4N. That indicates stability ofthe Fe4N phases with respective to elemental BCC-Fe metal andN2, in agreement with the experimental observations of thestable I-Fe4N phase.16,18,102 The small energy difference alsoindicates that the less stable II-Fe4N phase may be synthesizedat elevated temperature experimentally.
The calculations also showed that for M ¼ Co and Ni, theformation energies are positive with respect to the elementalsolids (HCP-Co and FCC-Ni) and N2 molecule The phasediagrams for Co–N106,107 and Ni–N108 show a stable M3N phaseand metastable M4N phase, in line with our calculations.Experimentally, I-Co4N samples were obtained by differentapproaches,19,20 and both I- and II-Ni4N were obtained by meansof nitridization of Ni metal at elevated experimentally.4,8,9
3.2d. M¼ Cu and Zn. Both elements have fully occupied 3dstates (3d10). The M4N phases are non-magnetic as shown inTable 2. Our calculations for I-Cu4N produced a lattice param-eter of about 3.877 A. There is only one experimental report on I-Cu4N samples prepared by DC plasma (ion) heating of coppersheet in a nitrogen and hydrogen atmosphere to 450 to 530 �C.21
The authors also reported their results of structural analysis.The cubic Cu4N phase has a lattice parameter of 3.193 A whichis much smaller than that of the present calculations, and evensmaller than the lattice parameter (3.615 A) of pure copper.68,69
However, our calculated lattice parameter (3.877 A) agrees withthe recent theoretical results (3.888 A).49,109 The too small latticeparameter obtained experimentally may originate from impu-rity of the samples, as Cu4N is calculated to be metastable orunstable with signicant higher formation energy with respectto the elemental Cu and nitrogen gas (Table 2). In order to havea better understanding about the stability and structural prop-erties of the M4N phases, we also performed calculations for thewell-known Cu3N phase with the anti-Re3O type structure.49,109
Our calculations produced a lattice parameter of 3.837 A, closeto the experimental value (3.819 A),110 and the former calcula-tions 3.846 (ref. 49) and (3.849 A).110 From the equation: Cu4N(s)¼ Cu (s) + Cu3N (s) + DHform, we obtained DHform ¼ +0.372 eV/f.u. for I-Cu4N and +0.537 eV/f.u. for II-type phase. Therefore,the Cu4N phases are metastable with respect to Cu metal andCu3N. For the Zn4N phases, the II-type is more stable than the I-Zn4N. However, both phases are metastable with respect to theelemental HCP-Zn and N2 molecule. In fact, zinc nitride isstable with a rather strict chemical composition Zn3N2. That isunderstandable since Zn atom behaves more like a normalmetal rather than a transition metal111,112 with the occupied 3dstates being regarded as semi-core.13,113
The 3d transition metal nitrides M4N also provide anopportunity to investigate chemical bonding and charges atatomic sites and charge-transfer between the 3d transitionmetals and nitrogen atoms/ions.114 As shown in Section 2.2, theBader approach can be used to determine unambiguously thecharge on atoms and the charge transfer in crystals.56–58 Theresults are shown in Fig. 4 and Table S1.†
7892 | RSC Adv., 2014, 4, 7885–7899
In chemistry, the electro-negativity c is an important param-eter and it describes the tendency of an atom to attract elec-trons.114,115 The difference Dc between two atoms indicates thedifference in capability to attract electrons. In other words, it isindicative of the charge transfer between atoms/ions in a crystal.At present there are two sets of electro-negativity parameters. Thewidely used ‘Pauling electro-negativity’ of elements was calcu-lated by Allred in 1981 with c listed in Table 2.116 In 1989, Allenpublished his set of electro-negativity values for elements.117
Fig. 4 includes the electro-negativity differences between themetallic atom and nitrogen atom: Dc ¼ c(M) – c(N). Fig. 4 showsthe Bader charge at different atomic sites in the M4N phases andthe Dc values for the two sets (Pauling scale and Allen scale).116,117
As shown in Fig. 4, the two curves of Dc values on atomicnumbers of the metal atoms in the M4N phases have verysimilar trends with exception for Mn: Dc increases and reach amaximum at Ni; and then decreases to M ¼ Zn.
Generally the charge Q(N) curves in I- and II-M4N are similarto those of Dc except for M ¼ Ti and Co. The Q(N) curve for I-M4N is below that of the II-phases. More interesting is thecharge at the metal sites (Fig. 4, top): the M1 atoms that are faraway (d(M1–N)¼ O3 ao/2) from the N atoms in I-M4N lose muchmore electrons, while the M2 atoms lose less, only about 1/3 to1/2 of the number of electrons lost by the M1 atoms. Please notethat the M1 atoms do not have any N atoms as nearest-neigh-bors. These results indicate strong interactions between the M1and M2 atoms. In the II-M4N phases, the M1 atoms lose moreelectrons than the corresponding M2 atoms, in accordance withthe fact that each M1 is connected to two N atoms while eachM2 atom is coordinated by only one N atom (Fig. 1 and Table 3).
3.3. Electronic and magnetic properties of M4N
We rst analyze the eigenvalues of M 3d states in the crystaleld of the FCC-lattice using M ¼ Ni as an example. At the G
This journal is © The Royal Society of Chemistry 2014
Paper RSC Advances
point in the Brillouin zone, the ve 3d orbitals split into twodegenerate states, triplet eg and doublet t2g. For NM Ni, thesplitting between t2g (lower in energy) and eg (higher in energy)is about 1.1 eV. Spin-polarization calculations produceexchange interaction energies of about 0.7 eV for eg and 0.6 eVfor the t2g band. The itinerant nature of Ni 3d states and s–dinteractions cause the large dispersion of the states.10–13
Therefore, there are no apparent peaks of the t2g and eg bands asshown in Fig. 5. In non-magnetic I-M4N (M ¼ Ni) the M1 3dstates form a narrow band between �1.0 to 0.5 eV with sometails between �4 and �1.0 eV. The M2 3d states have broadband with a width by about 4.5 eV, originating from the M2-Ninteractions. Therefore, the large charge loss at the M1 sites to Ntakes place via M1–M2 bonding. It is also notable that there arestrong overlaps between M1 and M2 in the energy range �4 to�1 eV, indicating strong interactions between M1 and M2 3dstates. In fact eigen-symmetry analysis for the lowest states ofthe Ni 3d states at G shows a doublet band with contributionsfrom both M1 and M2. For the II-type structures, the lowersymmetry and chemical bonds have reduced the degeneracy ofstates. The detailed partial DOS and total DOS curves for all theM4N phases are shown in Fig. 6(a–i) and are discussed in detailbelow.
As mentioned before, the electronic structure and magneticproperties of I-Fe4N have been carefully studied by rst-princi-ples methods.5–7,17,22–32 Kong and co-workers performed elec-tronic structure calculations for II-Fe4N by assuming lattices a¼a0 (lattice parameter of I-type structure) and c ¼ 2a.25 There arealso rst-principles studies on the electronic and magneticproperties of the I-M4N phases for M ¼ V.47 Mn,33,34 Co,35 Ni(ref. 41) and Cu.49,109
Fig. 5 shows a typical electronic structure of a (non-magnetic) M4N phase compared with FCC-M (M ¼ Ni asexample). The partial density of the Ni 3d states of the non-magnetic FCC-Ni solution is included for comparison. Thecharacteristics of the electronic properties and local electronic
Fig. 5 Schematic pDOS curves for M 3d states of a non-magnetic fcc-metal (top) and of M1 and M2 atoms in nonmagnetic I-M4N using M ¼Ni as the example.
This journal is © The Royal Society of Chemistry 2014
congurations and local magnetic moments in the atomicspheres with Wigner–Seitz radii of 1.40 A for metals and 1.00 Afor N are listed in Table S2 (ESI†). Details of the partial and totalDOS for the M4N phases are given in Fig. 6a–i. The overallelectronic structure for the M4N phases is composed of twoseparate parts: occupied N 2s states at about �16 eV with band-widths of about 1.0 to 2.5 eV and valence -conduction bandsstarting from about �8 eV below its Fermi level which is set atzero eV. The rather notable band widths of the N 2s statesindicate interactions between the semi-core N 2s electrons andother atoms. However, this interaction does not contribute tothe chemical bonding since both bonding and anti-bondingstates are occupied.
As shown in Fig. 5 and 6, the N 2p bands can be welldistinguished from the metal 3d states. The N 2p states are atthe bottom of the valence bands. The 2p electrons in one Nsphere (Wigner–Seitz radius of 1.0 A) are about 3.0 electrons(Table S2†). Note that the number of electrons at an atomic siteis strongly dependent on the size of the sphere. When a radiusof 1.32 A is used for N, the number of the 2p electrons at the Nsite becomes 4.12 electrons. As shown in Fig. 4, Bader chargeanalysis yields a charge of �2.5 to �1.5 electrons on the Natoms. This relates to the ionic nature of the M4N crystals.
As discussed above, the magnetism of the M4N phases hasbeen a subject of intensive research. Here we discuss themagnetism of the M4N phases in detail. As shown in Tables 2and 3 and Fig. 2 and 6, the I-M4N phases are magnetic for M ¼Cr to Ni, while II-Cr4N and II-Ni4N are non-magnetic. Fig. 7shows that I-Cr4N, I-Mn4N, and II-Mn4N are calculated to haveferri-magnetic ordering, while I-M4N with M¼ Fe, Co and Ni, aswell as II-Fe4N and II-Co4N are ferro-magnetic. Fig. 7a shows thedependence of local magnetic moments on the metal atoms. Inthe I-M4N phases, the M1 atoms have signicantly largermagnetic moments than the corresponding values at the M2atoms. That corresponds to the higher charges at the M1 atoms/ions in comparison to those in the M2 atoms of I-M4N phases,as shown in Fig. 4 and Table 3. Comparatively, the localmoments in II-M4N are more complex. While the Mn1 atoms inII-Mn4N have slightly larger magnetic moments than the cor-responding Mn2 atoms, the Fe1 and Co1 atoms have smallerlocal moments than that of the Fe2 and Co2 atoms as shown inTable 3 and Fig. 7a.
There are few publications about the magnetism of the M4Nphases, except for the case M¼ Fe where more studies have beenperformed. Our calculated local moments (3.40/�0.81 mB) forMn1/Mn2 atoms in I-Mn4N are close to the experimental values(3.85/�0.90 mB, respectively),98 and agree well with the formercalculations (3.23/�0.80 mB) by Mohn and co-workers using theatomic spherical wave approach.33,34 The calculated localmoment (2.97/2.35 mB/Fe) of the Fe1/Fe2 atoms in I-Fe4N, areclose to the experimental value (3.0/2.0 mB/Fe),1 as well as otherrst-principles calculations (2.98/1.79 mB/Fe,34 2.96/2.24 mB/Fe,17
2.98/2.23 mB/Fe (ref. 22)). The calculated local magnetic moments(1.96/2.54 mB/Fe) of the Fe1/Fe2 atoms in II-Fe4N also agree withthe former theoretical calculations (2.03/2.54 mB/Fe, respectively)by Kong and co-workers who assumed the lattice parameters a ¼a0 and c ¼ 2a0 (a0 is the lattice parameter of I-Fe4N).25 The
RSC Adv., 2014, 4, 7885–7899 | 7893
Fig. 6 Partial and total density of states for Sc4N (a), Ti4N (b), V4N (c), Cr4N (d), Mn4N (e), Fe4N (f), Co4N (g), Ni4N (h) and Cu4N (i) phases.
7894 | RSC Adv., 2014, 4, 7885–7899 This journal is © The Royal Society of Chemistry 2014
RSC Advances Paper
Fig. 7 (a) The absolute values of the local magnetic moments of themetal atoms in the M4N phases. (b) Relationship between the totalmagnetic moment and the number of 3d electrons in the ferromag-netic M4N phases (M ¼ Fe, Co, Ni and Cu), i.e. Slater–Pauling curve (b).The dotted lines are drawn to guide the eyes.
Fig. 8 Calculated |P| values for M1 (triangle-up) and M2 (triangle-down) atoms and the compounds (spheres) for I- (black) and II-M4N(red) (M ¼ Cr to Ni) phases. The P values with a negative sign arelabeled by open symbols instead of solid symbols. The dotted lines aredrawn to guide the eyes.
Paper RSC Advances
calculations for I-Co4N also reproduced the results by Mater andco-workers35 as shown in Table S2.†
The Slater–Pauling curves have been widely used to study therelationships between calculated magnetic moments and thenumber of 3d electrons for alloys118,119 and half-metals,120 as wellas for for the compounds I-(Fe, Co)4N the Fe4N–Co4N system.6
Fig. 7b shows the Slater–Pauling curve for the ferro-magneticM4N phases. The total magnetic moments in I-M4N decreasewith increasing number of 3d electrons. That corresponds tothe rigid band lling for the electronic structure of almost fullyoccupied 3d states for majority electrons. It is also clear that themagnetic moments of the II-M4N phases decrease rapidly withincreasing number of 3d electrons, probably due to the localchemical bonding and distortion of the FCC-metal sub-lattices.As shown in Fig. 6g, the densities of Co1/Co2 3d states at theFermi level for the spin-up (majority) electrons are extremelylow, and high for the spin-down electrons. That corresponds tothe nearly half-metallic nature rst obtained by Takahashi andco-workers.6
To have a clear picture about the capability of spin-carriersfor the M4N phases, we used the denition of spin-polarizationratio P:
P ¼ [D[(3F) � DY(3F)]/[D[(3F) + DY(3F)] (5)
Where D[(3F)/DY(3F) represents the density of states of an atom/
ions or a compound at Fermi level for the spin-up/spin-downelectrons, respectively. For pure half metallic materials, such assemi-Heusler NiMnSb36,40 which is metallic for spin-up elec-trons (D[(3F)s 0) and semi-conducting for spin-down electrons(DY(3F) ¼ 0), then P ¼ 1.0 (or 100%). Meanwhile for non-magnetic materials, D[(3F) ¼ DY(3F), and consequently P ¼ 0.0.The calculated spin-polarization ratios of the M1 and M2 atomsin the M4N phases and the P for the compounds are shown in
This journal is © The Royal Society of Chemistry 2014
Fig. 8. For sake of comparison, we only show the absolute Pvalues (the negative ones are indicated with open symbols).
From the combination of Fig. 6 and 8, the P values for II-M4Nare generally much lower than those of the corresponding I-phases. It is notable that the P values of the total DOS for II-M4Nare considerably lower than those of the atoms, partially due tothe contributions of N 2p states at the Fermi level (see Table 3).The absolute P values of the M1 atoms/ions in I-M4N (M ¼ Cr toNi) phases are much higher than those of the corresponding M2atoms/ions. The P values are over 90% for I-M4N (M ¼ Mn, Feand Co) and near 87% for M ¼ Ni. In contrast, the low values ofthe M2 atoms/ions cause the P values of the compounds to bemuch lower, 50 to 60% for M ¼ Mn, Fe and Ni, but still to 83%for M ¼ Co. The sign of the P value for Cr1 atoms is opposite tothat of Cr2 atoms. As a consequence, the P value of I-Cr4Nbecomes rather small (about 17.4%). The high P values of M1atoms in the I-M4N phases also provide the possibility to designnew phases exhibiting high P values for potential applicationsin spintronics.6,38,40
3.4. Origin of the magnetism and phase stability of M4N
In the 1930s, Stoner investigated the relationship between theexchange interaction and kinetic contribution for a bandstructure and proposed the well-known Stoner criterion:50,121,122
I$D(3F) $ 1 (6)
Where D(3F) is the density of states at the Fermi level (3F). TheStoner parameter which is a measure of the strength of theexchange correlation is denoted I. Brooks performed rst-principles calculations and obtained the Stoner parameters I forthe many transition metals, including 3d transition metals12 asshown in Table S2.†
RSC Adv., 2014, 4, 7885–7899 | 7895
RSC Advances Paper
Fig. 5 shows the calculated partial density (pDOS) of Ni 3dand N 2p states in a (nonmagnetic) FCC-metal (Ni as theexample) and nonmagnetic I-M4N (M ¼ Ni). As shown in Fig. 6,the pDOS curves for the M4N phases are very similar to the non-magnetic solution (Fig. 5). Therefore, we can estimate theelectronic structure for different 3d metals using the electronlling approach (a rigid model). However, to have accurateresults, we performed structural optimizations and electronicstructure calculations for the non-magnetic I-M4N phases andthe related (non-magnetic) FCC-metals. The calculated partialdensity of Ni 3d states are shown in Fig. 5 (top). The term I$D(3F)for each 3d metals is also shown in Fig. 9 (bottom) which showsthat FCC-Sc has rather high D(3F) for 3d electrons, corre-sponding to the electron conguration Sc 3d1 4s2. That is alsotrue for I-Sc4N. With increasing atomic number for the FCC-metal the value of D(3F) value increases, except for a small dip atMn, and reach a maximum at Ni. D(3F) has a very small value forFCC-Cu, in agreement with the Cu 3d104s2 electron congura-tion. The D(3F) values for M 3d states in the I-M4N phases havedifferent behaviors: D(3F) for M1 3d states increases smoothlyfrom Sc to V, then quickly from Cr and reach maximum at Feand Co nally fall to Cu; meanwhile D(3F) for M2 3d states rstincreases smoothly from Sc to Cr. There is a valley for M ¼ Mn.Then it increases again from Fe and reached a maximum forM ¼ Co.
The Stoner curves, I$D(3F) shown at the bottom of Fig. 9 showstrong similarity with the D(3F) curves for the M 3d electrons.Apparently for M ¼ Sc and Ti, all the three curves are below 1.For M ¼ V, the I$D(3F) values are close to 1, especially for V1 3dstates in I-V4N. Then from Cr to Ni, all the curves are above 1except for Mn2 atoms in I-Mn4N. In fact as shown in Table 3, in
Fig. 9 Calculated density of states at the Fermi level, D(3F) (a) and theI$D(3F) values (b), for non-magnetic FCC 3d transiton metals (openblack circles), M1 (solid red squares) and M2 (solid green diamonds) inthe I-M4N phases. The dashed line with values being equal to 1 rep-resented the Stoner criteria for instability of the nonmagnetic FCCmetal lattices. I$D(3F) < 1 indicates that the non-magnetic solution ismore stable while I$D(3F) > 1 indicates possible transitions: spin-polarization or John-Teller-like crystal-field distortions. The Stonerparameters I are listed in Table S2.†
7896 | RSC Adv., 2014, 4, 7885–7899
I-Mn4N the Mn1 atom has a very large magnetic moment of 3.4mB, while the Mn2 atoms have only a small moment (�0.8 mB)which can be considered to be induced by the Mn1 atoms. It canbe concluded that the Stoner criterion works well for the I-M4Nphases.
For the II-M4N phases, from Mn to Ni, the metal/atoms ionsexhibit magnetism. In contrast to the I-type structure, II-Cr4Nand II-Ni4N are non-magnetic. Former calculations for Naddition in FCC-Ni lattice showed that lattice distortion has astrong impact on the magnetism. While I-M4N is magnetic,chemical changes II-Ni4N1�x (with x � 0.03) cause local distor-tion and the defective phases becomes non-magnetic.41 That isalso the case for II-Ni4N.
Another possibility to reduce the DOS at the Fermi level isprovided by the Jahn–Teller theorem.123,124 The high symmetryof the FCC metal sub-lattices in I-M4N causes degenerate 3dstates, and consequently a high density of states at the Fermilevel (Fig. 8). The high DOS at the Fermi level causes theinstability of the structure, which can lead to two possibleeffects. The rst possibility is spin-polarization splitting ormagnetism due to exchange interaction (Stoner effects). Thesecond possibility is the distortion of the high-symmetry metalsub-lattice. And indeed, the metal sub-lattices in the II-M4Nphases are distorted due to the different c/a ratio, which willreduce the degeneracy of the metal 3d states as well as the pDOSat the Fermi level. According to Fig. 8, the competition betweenmagnetism and lattice distortion leads to higher stability of thenon-magnetic II-Cr4N and II-Ni4N phases.
4. Conclusions
We performed rst-principles calculations to predict in asystematic way the formation, stability and structures of theM4N phases using density-functional theory with generalizedgradient approximation. Bader charge analysis and electronicband structure calculations were performed for all 3d transitionmetal M4N phases. The calculations showed that high stabilityof the II-M4N (M ¼ Sc and Ti) phases over the corresponding I-type structures, originating from lattice relaxations and localchemical bonding between the M2 and N atoms. The predictedcrystal structures and the obtained magnetic moments agreewell with the available experimental data and former theoreticalcalculations. Bader charge analysis revealed the highly ionicnature of the compounds. Considering the small differences information energies, the calculations also predict that two M4Nphases may be synthesized experimentally, e.g., by formation atelevated temperatures, by growth on a suitable substrate, or asnano-sized crystals. The predicted crystal structures can beuseful for experimentalists to characterize the phases inprepared samples (thin lms, coated layers, nano-sized parti-cles, etc.), in particular because N is such a light atom thatdifferent N orderings are hard to distinguish experimentally.Electronic structure calculations showed strong interactionsbetweenM2 and N atoms, as well as metal–metal interactions inthe phases. Remarkably, the M1 atoms in the I-type phases loseelectrons to the N ions, though they do not have N atoms asnearest neighbors. Magnetism was observed for M4N with
This journal is © The Royal Society of Chemistry 2014
Paper RSC Advances
M ¼ Cr to Ni. While ferrimagnetic solutions were found for I-Cr4N, I-Mn4N, and II-Mn4N, ferro-magnetism was found for M¼ Fe to Ni. It is also notable that II-Cr4N and II-Ni4N are non-magnetic due to the distortion of the FCC-metal sub-lattices,and chemical bonding. Finally, high spin-polarization ratioswere found for the M1 atoms in I-M4N from M ¼ Mn to Ni. Thecalculated results are helpful to design new compounds ofdesirable physical properties.
Acknowledgements
We thank Prof. Dr Alfons van Blaaderen for his careful readingand encouragements. MvH acknowledges a VIDI grant from theDutch Science Foundation NWO.
Notes and references
1 B. C. Frazer, Phys. Rev., 1958, 122, 751.2 S. Suzuki, H. Sakumoto, J. Minegismi and Y. Omote, IEEETrans. Magn., 1981, 17, 3017.
3 H. Jia, X. Wang, W. T. Zheng, Y. Chen and S. H. Feng,Mater.Sci. Eng., B, 2008, 150, 121.
4 A. I. Linnik, A. M. Prudnikov, R. V. Shalav, T. A. Linnik,V. N. Varyukhin, S. A. Kostyrya and V. V. Burkhovetskii,Phys. Lett., 2013, 39, 143.
5 J. L. Costa-Kramer, D. M. Borsa, J. M. Garcıa-Martın,M. S. Martın-Gonzalez, D. O. Boema and F. Briones, Phys.Rev. B: Condens. Matter Mater. Phys., 2004, 69, 144402.
6 Y. Takahashi, Y. Imai and T. Kumagai, J. Magn. Magn.Mater., 2011, 323, 2941.
7 P. Dhanasekaran, H. G. Salunke and N. M. Gupta, J. Phys.Chem. C, 2012, 116, 12156.
8 N. Terao, Naturwissenschaen, 1958, 45, 620, (I-Ni4N).9 N. Terao, J. Phys. Soc. Jpn., 1960, 15, 227, (II-Ni4N).10 C. Herring, J. Appl. Phys. Suppl., 1960, 31, 3S.11 S. Asano and J. Yamashita, Prog. Theor. Phys., 1973, 49, 373.12 M. S. S. Brooks, in Conduction electrons in magnetic metals,
in Magnetism in Metals, ed. D. F. McMorrow, J. Jensen andH. M. Rønnow, Det Kongelige Danske VidenskabernesSelskab, Denmark, 1997, p. 291.
13 N. F. Mott, Proc. Phys. Soc., London, Sect. A, 1949, 62, 416.14 O. Gunnarsson and K. Schonhammer, Phys. Rev. Lett., 1983,
50, 604.15 J. Zaanen, G. A. Sawatzky and J. W. Allen, Phys. Rev. Lett.,
1985, 55, 418.16 K. H. Jack, Acta Crystallogr., 1952, 5, 404.17 X. G. Ma, J. J. Jiang, P. Liang, J. Wang, Q. Ma and
Q. K. Zhang, J. Alloys Compd., 2009, 480, 475.18 H. Jacobs, D. Rechenbach and U. Zachwieja, J. Alloys
Compd., 1995, 227, 10.19 X. Wang, H. Jia, W. T. Zheng, Y. Chen and S. H. Feng, Thin
Solid Films, 2009, 517, 4419.20 K. Ito, K. Harazunori, K. Toko, H. Akinaga and T. Suemasu,
J. Cryst. Growth, 2011, 336, 40.21 J. Blucher, K. Band and B. C. Giessen, Mater. Sci. Eng., A,
1989, 117, L1.
This journal is © The Royal Society of Chemistry 2014
22 R. Coehoorn, G. H. O. Daalderop and H. J. F. Jansen, Phys.Rev. B: Condens. Matter Mater. Phys., 1993, 48, 3830.
23 M. Neklyudov and A. N. Morozov, Physica B, 2004, 350, 325.24 S. Kokado, N. Fujima, K. Harigaya, H. Shimizu and
A. Sakuma, Phys. Status Solidi B, 2006, 3, 3303.25 Y. Kong, J. Pelzl and F. S. Li, J. Magn. Magn. Mater., 1999,
195, 483.26 B. Eck, R. Dronskowski, M. Takahashi and S. Kikkawa, J.
Mater. Chem., 1999, 9, 1527.27 N. Timoshevskii, V. A. Timoshevskii, B. Z. Yanchitsky and
V. A. Yavna, Comput. Mater. Sci., 2001, 22, 99.28 S. Kodado, N. Fujima, K. Harigaya, H. Shimizu and
A. Sakuma, Phys. Rev. B: Condens. Matter Mater. Phys.,2006, 73, 172410.
29 T. Gressmann, M. Wohlschlogel, S. Shang, U. Welzel,A. Leineweber, E. J. Mittemeijer and Z. K. Liu, Acta Mater.,2007, 55, 5833.
30 D. Li, K. Roh, K. J. Jeon, Y. S. Gu and W. Lee, Phys. StatusSolidi B, 2008, 245, 2581.
31 J. Yang, H. Sun and C. F. Chen, Appl. Phys. Lett., 2009, 94,151914.
32 Z. Q. Lv, Y. Gao, S. H. Sun, M. G. Qv, Z. H. Wang, Z. P. Shiand W. T. Fu, J. Magn. Magn. Mater., 2013, 333, 39.
33 B. Siberchicor and S. Matar, J. Magn. Magn. Mater., 1991,101, 419.
34 P. Mohn, S. Matar, G. Demazeau and E. P. Wohlfarth, J.Phys., Colloq., 1988, 8, 95.
35 S. F. Matar, A. Houari and M. A. Belkhir, Phys. Rev. B:Condens. Matter Mater. Phys., 2007, 75, 245109.
36 R. A. de Groot, F. M. Muller, P. O. Van Engen andK. H. Buschow, J. Phys. Rev. Lett., 1983, 50, 2024.
37 J. H. Park, E. Vescova, H. J. Kim, C. Kwon, R. Ramesh andT. Venkatesan, Nature, 1998, 392, 794.
38 W. E. Pickett and J. S. Moodera, Phys. Today, 2001, 54,39.
39 S. A. Wolf, D. D. Awschalom, R. A. Buhrman, J. M. Daughton,S. von Molnar, M. L. Roukes, A. Y. Chtchelkanova andD. M. Treger, Science, 2001, 294, 1488.
40 C. M. Fang, G. A. de Wijs and R. A. de Groot, J. Appl. Phys.,2002, 91, 8340.
41 C. M. Fang, M. H. F. Sluiter, M. A. van Huis andH. W. Zandbergen, Phys. Rev. B: Condens. Matter Mater.Phys., 2012, 86, 134114.
42 J. Zhao, H. P. Xiang, J. Meng and Z. J. Wu, Chem. Phys. Lett.,2007, 449, 96.
43 Z. J. Wu and J. Meng, Appl. Phys. Lett., 2007, 90, 241901.44 A. Houben, J. Burghaus and R. Dronskowski, Chem. Mater.,
2009, 21, 4332.45 J. Burghaus, M. Wessel, A. Houben and R. Dronkskowski,
Inorg. Chem., 2010, 49, 10148.46 T. Woehrle, A. Leineweber and E. J. Mittermeijer, Metall.
Mater. Trans. A, 2012, 43, 610.47 A. V. dos Santos, J. C. Krause and C. A. Kuhnen, Physica B,
2006, 382, 290.48 J. G. Niu, W. Gao, X. P. Dong, L. Guan and F. Xie, Adv. Mater.
Res., 2010, 150–151, 1290.49 Z. F. Hou, Solid State Sci., 2008, 10, 1651.
RSC Adv., 2014, 4, 7885–7899 | 7897
RSC Advances Paper
50 E. C. Stoner, Proc. R. Soc. London, Ser. A, 1938, 165, 372.51 D. M. Edwards and E. P. Wohlfarth, Proc. R. Soc. London,
Ser. A, 1968, 303, 127.52 R. Niewa and F. J. DiSalvo, Chem. Mater., 1998, 10, 2733.53 J. W. Christian, The theory of transformation in metals and
alloys, Pergamon Press, Amsterdam/Boston/London/NewYork/Oxford/Paris/San Diego/San Francisco/Singapore/Sydney/Tokyo, 2002.
54 C. M. Fang, M. A. van Huis, M. H. F. Sluiter andH. W. Zandbergen, Phys. Rev. Lett., 2010, 105, 055503.
55 C. Domain, C. S. Becquart and J. Foct, Phys. Rev. B: Condens.Matter Mater. Phys., 2004, 69, 144112.
56 R. F. W. Bader and P. M. Beddal, Chem. Phys. Lett., 1971, 8, 29.57 R. F. W. Bader, T. T. Nguyen and Y. Tal, Prog. Phys., 1981, 44,
893.58 G. Henkelman, A. Arnaldsson and H. Jonsson, Comput.
Mater. Sci., 2006, 36, 254.59 G. Kresse and J. Hafner, Phys. Rev. B: Condens. Matter Mater.
Phys., 1993, 47, 558.60 G. Kresse and J. Furthmuller, Comput. Mater. Sci., 1996, 6,
15.61 C. M. Fang, M. A. van Huis, J. Jansen and
H. W. Zandbergen, Phys. Rev. B: Condens. Matter Mater.Phys., 2011, 84, 094102.
62 P. E. Blochl, Phys. Rev. B: Condens. Matter Mater. Phys., 1994,50, 17953.
63 G. Kresse and J. Furthmuller, Phys. Rev. B: Condens. MatterMater. Phys., 1999, 54, 1758.
64 J. P. Perdew, K. Burke and M. Ernzerhof, Phys. Rev. Lett.,1996, 77, 3865.
65 C. Amador, W. R. Lambrecht and B. Segall, Phys. Rev. B:Condens. Matter Mater. Phys., 1992, 46, 1870.
66 C. M. Fang, M. A. van Huis, M. H. F. Sluiter andH. W. Zandbergen, Acta Mater., 2010, 58, 2968.
67 H. J. Monkhorst and J. F. Pack, Phys. Rev. B: Solid State,1976, 13, 5188.
68 R. W. G. Wyckoff, Crystal Structures, Intersciences, NewYork, NY, 1964.
69 There are many summaries for the symmetry and latticeparameters of elemental metals, e.g. http://www.perionictable.com/Elements.
70 L. Corliss, J. Hastings and R. Weiss, Phys. Rev. Lett., 1959, 3,211.
71 R. Soulairol, C. C. Fu and C. Barreteau, Phys. Rev. B:Condens. Matter Mater. Phys., 2011, 8, 214103.
72 A. C. Lawson, A. C. Larson, M. C. Aronson, S. Johnson,Z. Fisk, P. C. Caneld, J. D. Thompson and R. B. VonDreele, J. Appl. Phys., 1994, 76, 7049.
73 N. N. Greenwood and A. Earnshaw, Chemistry of theElements, Butterworth-Heinemann, ISBN 0080379419, 2ndedn, 1997, p. 240.
74 V. Iota, J. H. P. Klepeis, C. S. Yoo, J. Lang, D. Haskel andG. Srajer, Appl. Phys. Lett., 2007, 90, 042505.
75 D. Hobbs, J. Hafner and D. Sposak, Phys. Rev. B: Condens.Matter Mater. Phys., 2003, 68, 014407.
76 B. Predel, Co–N (Cobalt–Nitrogen), ed. O. Madelung,SpringerMaterials – The Landolt-Bornstein Database,
7898 | RSC Adv., 2014, 4, 7885–7899
http://www.springermaterials.com, DOI: 10.1007/10086082_928.
77 E. Fawcett, Rev. Mod. Phys., 1988, 60, 209.78 G. Wright and J. Goddard, Philos. Mag., 1965, 11, 485.79 P. Wicksted, G. Shirane and O. Steinsvoll, J. Appl. Phys.,
1984, 55, 1893.80 G. A. Prinz, Phys. Rev. Lett., 1985, 54, 1051.81 S. Yoo, H. Cynn, P. Soderlind and V. Iota, Phys. Rev. Lett.,
2000, 84, 4132.82 W. Lengauer, J. Solid State Chem., 1988, 76, 412.83 Z. Gu, J. H. Edgar, J. Pomeroy, M. Kuball and D. W. Coffey, J.
Mater. Sci.: Mater. Electron., 2004, 15, 555.84 H. Okamoto, J. Phase Equilib., 1993, 14, 536, N–Ti (nitrogen–
titanium).85 H. Okamoto, J. Phase Equilib. Diffus., 2013, 34, 151, N–Ti
(nitrogen–titanium).86 S. Nagakura, T. Kusunoki, F. Kakimoto and Y. Hirotsu,
J. Appl. Crystallogr., 1975, 8, 65.87 N. Christensen, Acta Crystallogr., Sect. C: Cryst. Struct.
Commun., 1985, 41, 1009.88 W. Lengauer, Acta Metall. Mater., 1991, 39, 2985.89 G. K. Tirumalasetty, M. A. van Huis, C. M. Fang, Q. Xu,
F. C. Tichelaar, D. N. Hanlon, J. Sietsma andH. W. Zandbergen, Acta Mater., 2011, 59, 7406.
90 N. Carlson, J. F. Smith and R. H. Nafziger, Metall. Mater.Trans. A, 1986, 17, 1847.
91 H. Okamoto, J. Phase Equilib. Diffus., 1994, 15, 454,Comment on N–V (nitrogen–vanadium).
92 M. Enomoto, J. Phase Equilib. Diffus., 1996, 17, 248, The N–Ti–V system (nitrogen–titanium–vanadium).
93 N. Christensen and B. Lebech, Acta Crystallogr., Sect. B:Struct. Crystallogr. Cryst. Chem., 1979, 35, 2677.
94 K. Frisk, CALPHAD: Comput. Coupling Phase DiagramsThermochem., 1991, 15, 79.
95 V. G. Ivanchenko and T. V. Mel'nichenko, Metallozika,1991, 13, 23.
96 M. Aoki, H. Yamane, M. Shimada and T. Kajiwara, J. Cryst.Growth, 2002, 246, 133.
97 N. A. Gokcen, Bull. Alloy Phase Diagrams, 1990, 11, 33.98 W. J. Takei, R. R. Heikes and G. Shirane, Phys. Rev., 1962,
125, 1893.99 M. Hillert, L. Hoglund and J. Agren, J. Appl. Phys., 2005, 98,
053511.100 N. Mryasov, V. A. Gubanov and A. I. Liechtenstein, Phys.
Rev. B: Condens. Matter Mater. Phys., 1992, 45, 12330.101 K. Oda and H. Ino, J. Phys.: Condens. Matter, 1990, 2,
10147.102 J. Kool, M. A. J. Somers and E. J. Mittemeijer,Metall. Mater.
Trans. A, 1996, 27, 1061.103 N. Terao, Mem. Sci. Rev. Metall., 1960, 57, 96.104 K. Ito, K. Harada, K. Toko, H. Akinaga and T. Suemasu, J.
Cryst. Growth, 2011, 336, 40.105 K. Oda, K. Kenichi and I. Takashi, J. Mater. Sci., 1987, 22,
2729.106 V. Raghavan, J. Phase Equilib., 1993, 14, 623, Co–Fe–N
(Cobalt–Iron–Nitrogen).107 R. Juza and W. Sachsze, Z. Anorg. Chem., 1945, 253, 95.
This journal is © The Royal Society of Chemistry 2014
Paper RSC Advances
108 H. A. Wriedt, Bull. Alloy Phase Diagrams, 1985, 6, 558, TheN–Ni (nitrogen–nickel) system.
109 X. Y. Cui, A. Soon, A. E. Phillips, R. K. Zheng, Z. W. Liu,B. Delley, S. P. Ringer and C. Stamp, J. Magn. Magn.Mater., 2012, 324, 3138.
110 U. Zachwiecha and H. Jacobs, J. Less-Common Met., 1990,161, 175.
111 H. A. Wriedt, Bull. Alloy Phase Diagrams, 1988, 9, 247, TheN–Zn (nitrogen–zinc) system.
112 M. Futsuhara, K. Yoshioka and O. Takai, Thin Solid Films,1998, 322, 274.
113 C. Persson and A. Zunger, Phys. Rev. B: Condens. MatterMater. Phys., 2003, 68, 073205.
114 L. Pauling, J. Am. Chem. Soc., 1932, 54, 3570.115 G. Frenking and N. Frohlich, Chem. Rev., 2000, 100, 717.
This journal is © The Royal Society of Chemistry 2014
116 L. Allred, J. Inorg. Nucl. Chem., 1961, 17, 215.117 L. C. Allen, J. Am. Chem. Soc., 1989, 111, 9003.118 Y. Kakehashi and O. Hosohata, J. Phys., Colloq., 1988,
8, 73.119 M. Shaughnessy, L. Damewood, C. Y. Fong, L. H. Yang and
C. Felser, J. Appl. Phys., 2013, 113, 043709.120 I. Galanakis, P. H. Dederichs and N. Papanikolaou, Phys.
Rev. B: Condens. Matter Mater. Phys., 2002, 66, 174429.121 E. C. Stoner, Proc. R. Soc. London, Ser. A, 1936, 154,
656.122 E. C. Stoner, Proc. R. Soc. London, Ser. A, 1939, 169, 339.123 H. Jahn and E. Teller, Proc. R. Soc. London, Ser. A, 1937, 161,
220.124 M. E. Eberhart, K. H. Johnson, D. Adler, R. C. O'Handley
and M. E. Mchenry, J. Non-Cryst. Solids, 1985, 75, 97.
RSC Adv., 2014, 4, 7885–7899 | 7899